IEC 60317-19 pdf download Specifications for particular types of winding wires – Part 19: Solderable polyurethane enamelled round copper wire, overcoated with polyamide, class 130
This International Standard specifies the requirements of solderable enamelled round copperwinding wire of class 130 with a dual coating.The underlying coating is based on polyurethane resin, which may be modified providing it retains the chemical identity of theoriginal resin and meets all specified wire requirements.The superimposed coating is basedon polyamide resin.
NOTE A modified resin is a resin that has undergone a chemical change, or contains one or more additives toenhance certain performance or application characteristics.
Class 130 is a thermal class that requires a minimum temperature index of 130 and a heatshock temperature of at least 155C.
The temperature in degrees Celsius corresponding to the temperature index is not necessarilythat at which it is recommended that the wire be operated and this will depend on many
factors, including the type of equipment involved.
The range of nominal conductor diameters covered by this standard is:-Grade 1: 0,050 mm up to and including 1,600 mm;
– Grade 2: 0,050 mm up to and including 2,000 mm.
The nominal conductor diameters are specified in clause 4 of lEC 60317-O-1.
The following standard contains provisions which, through reference in this text, constituteprovisions of this International Standard.At the time of publication, the edition indicated wasvalid.All standards are subject to revision,and parties to agreements based on this
International Standard are encouraged to investigate the possibility of applying the most
recent edition of the standard indicated below.Members of lEC and lSO maintain registers ofcurrently valid international standards.
IEC 60317-0-1:1990, Specifications for particular types of winding wires – Part 0:Generalrequirements – Section 1: Enamelled round copper wire
3Definitions and general notes on methods of test
For definitions and general notes on methods of test, see clause 3 of lEC 60317-0-1.
In case of inconsistencies between IEC 60317-O-1 and this standard, IEC 60317-19 shallprevail.
See clause 4 of lEC 60317-O-1.
See clause 5 of lEC 60317-O-1.
See clause 6 of IEC 60317-O-1.
See clause 7 of IEC 60317-O-1.
8Flexibility and adherence
See clause 8 of lEC 60317-O-1, where the constant K used for the calculation of the numberof revolutions for the peel test shall be 150 mm.
See clause 9 of lIEC 60317-0-1, where the minimum heat shock temperature shall be 155 ℃.
No failure shall occur within 2 min at 170C.
11 Resistance to abrasion (nominal conductor diameters from 0,250 mm up to and including 2,000 mm)
The wire shall meet the requirements given in table 1.